- About this Journal ·
- Abstracting and Indexing ·
- Advance Access ·
- Aims and Scope ·
- Annual Issues ·
- Article Processing Charges ·
- Articles in Press ·
- Author Guidelines ·
- Bibliographic Information ·
- Citations to this Journal ·
- Contact Information ·
- Editorial Board ·
- Editorial Workflow ·
- Free eTOC Alerts ·
- Publication Ethics ·
- Reviewers Acknowledgment ·
- Submit a Manuscript ·
- Subscription Information ·
- Table of Contents

Journal of Nanomaterials

Volume 2013 (2013), Article ID 371356, 8 pages

http://dx.doi.org/10.1155/2013/371356

## Semiconductor Photocatalyst: Possibilities and Challenges

Department of Applied Physics, Key Laboratory for Micro-Nano Physics and Technology of Hunan Province, Hunan University, Changsha 410082, China

Received 30 January 2013; Accepted 8 March 2013

Academic Editor: Yongzhu Fu

Copyright © 2013 Gui-Fang Huang et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

Ag_{3}PO_{4} as a photocatalyst has attracted enormous attention in recent years due to its great potential in harvesting solar energy for environmental purification and fuel production. The photocatalytic performance of Ag_{3}PO_{4} strongly depends on its morphology, exposed facets, and particle size. The effects of morphology and orientation of Ag_{3}PO_{4} on the catalytic performance and the efforts on the stability improvement of Ag_{3}PO_{4} are reviewed here. This paper also discusses the current theoretical understanding of photocatalytic mechanism of Ag_{3}PO_{4}, together with the recent progress towards developing Ag_{3}PO_{4} composite photocatalysts. The crucial issues that should be addressed in future research activities are finally highlighted.

#### 1. Introduction

The development of efficient photocatalysts is very important and desirable in environmental pollution mediation and solar energy conversion [1–6]. Over the past decades, fundamental progress has been made in developing novel photocatalysts, particularly visible light response catalysts for the efficient utilization of solar energy. A great deal of photocatalysts, including inorganic, molecular, and hybrid organic/inorganic materials, have been explored to meet specific requirements such as a light-absorbing wavelength modification, photoinduced charge separation, and a faster photocatalytic reaction. Among the various photocatalysts developed, TiO_{2} is undoubtedly the most popular and widely used photocatalyst since it is of low cost, high photocatalytic activity, chemical and photochemical stability [7, 8]. However, TiO_{2} is not ideal for all purposes and performs rather poorly in processes associated with solar photocatalysis due to its wide band gap (3–3.2 eV), thus making impractical overall technological process based on TiO_{2}. To design visible-light-driven photocatalysts, two strategies have been proposed. One is to modify the wide band gap photocatalysts (such as TiO_{2}, ZnS) by doping or by producing hetero-junctions between them and other materials [4, 7–12], and the other involves exploration of novel semiconductor materials capable of absorbing visible light. Various compounds, such as BiVO_{4} [13], Bi_{2}WO_{6} [1, 14], CaBi_{2}O_{4} [15], PbBi_{2}Nb_{2}O_{9} [16], Bi_{4}Ti_{3}O_{12} [17], and Ag@AgCl [18], and others have been reported to be promising photocatalysts under visible light irradiation [19–22]. Despite many of these photocatalysts being effective for the degradation of organic pollutants and water splitting, up to date, the present achievements are still far from the ideal goal.

Yi and his coworkers [23] have recently presented the pioneering work on exploring the photocatalytic properties of Ag_{3}PO_{4} that exhibit extremely high photooxidative capabilities for the O_{2} evolution from water and the decomposition of organic dyes under visible-light irradiation. Actually, the photodegradation rate of organic dyes over Ag_{3}PO_{4} is dozens of times faster than the rate over BiVO_{4} and commercial TiO_{2−x}N_{x} [23, 24]. Moreover, the most interesting is that this novel photocatalyst can achieve a quantum efficiency of up to 90% at wavelengths greater than 420 nm, which is significantly higher than the previous reported values. This finding potentially opens an avenue for solving current energy crisis and environment problems with abundant solar light, and the research of Ag_{3}PO_{4} is thus attracting considerable interest. Since then, many efforts have been devoted to further improving and optimizing their photoelectric and photocatalytic properties. Despite the fact that Ag_{3}PO_{4} is a promising candidate for environmental remediation and renewable energy, the consumption of a large amount of noble metal and the low structural stability of pure Ag_{3}PO_{4} strongly limits its practical environmental applications. Therefore, it is a highly crucial task to improve the photocatalytic stability of Ag_{3}PO_{4} while maintaining its high photocatalytic activity. In this paper, the effects of morphology and orientation of Ag_{3}PO_{4} on the catalytic performance and the current theoretical understanding of key aspects of Ag_{3}PO_{4} photocatalysts are presented. Also reviewed is the effort on the photocatalytic stability of Ag_{3}PO_{4} and Ag_{3}PO_{4} composite photocatalyst.

#### 2. The Structure of Ag_{3}PO_{4}

Ag_{3}PO_{4} is of body-centred cubic structure type with space group P4-3n and a lattice parameter of ~6:004 Å. The structure consists of isolated, regular PO_{4} tetrahedra (P–O distance of ~1.539 Å) forming a body-centred-cubic lattice. The six Ag^{+} ions are distributed among twelve sites of twofold symmetry [25]. This indicates that each Ag atom at (0.25, 0, 0.50) actually occupies one of the two sites at (, 0, 0.50) and (, 0, 0.50) on the 2-fold axis. The unit-cell structure of cubic Ag_{3}PO_{4} is shown in Figure 1, in which the Ag atom experiences 4-fold coordination by four O atoms [24]. The P atoms have 4-fold coordination surrounded by four O atoms, while the O atoms have 4-fold coordination surrounded by three Ag atoms and one P atom.

#### 3. Morphology Control and Catalytic Properties of Ag_{3}PO_{4}

Since Ag_{3}PO_{4} was first reported as visible light response photocatalyst by Yi and his coworkers [23], much research has been devoted to investigate this active photocatalyst [26–29], and different methods have been developed to synthesize various Ag_{3}PO_{4} and its composites [28, 30–32]. The investigation of photocatalytic activity shows that all of the prepared Ag_{3}PO_{4} exhibit excellent photocatalytic activity under UV light irradiation or visible-light illumination, which is much more excellent than that of commercial P25 TiO_{2} [33, 34] or N-doped TiO_{2} [30, 35, 36] as shown in Figure 2.

It is well known that the morphology of materials is closely related to the exposed facets of the crystals, which directly affect the properties of the catalysts. Various Ag_{3}PO_{4} nanostructures including spherical morphology [33, 34], rhombic dodecahedrons [30], concave trisoctahedrons [37], cubes [26, 30], and tetrapods [38] with controlling particle size [39] have been designed and synthesized to further improve or optimize the photocatalytic properties. The investigations revealed that the rhombic dodecahedrons exhibit much higher photocatalytic activity in comparison with spheres and cubes for the degradation of organic contaminants [23, 30], and the enhanced photocatalytic activity of Ag_{3}PO_{4} rhombic dodecahedrons is primarily ascribed to the higher surface energy of facets (1.31 J/m^{2}). The highly exposed facets also lead to the higher visible light activity of Ag_{3}PO_{4} tetrapods than that of the polyhedrons for the degradation of toxic organic compounds [38]. The concave trisoctahedral Ag_{3}PO_{4} microcrystals with high-index facets have also been reported to show much higher photocatalytic properties than cubic Ag_{3}PO_{4} and commercial N-doped TiO_{2} [37].

The synthetic parameters, such as reaction component, temperature, and reaction time, usually serve as effective routes for tailoring the morphology and structure of Ag_{3}PO_{4} crystals. By directly reacting AgNO_{3} and Na_{2}HPO_{4}, only Ag_{3}PO_{4} particles with irregular spherical structures can be obtained, while the single crystalline Ag_{3}PO_{4} submicrocubes with sharp corners, edges, and smooth surfaces can be fabricated with [Ag(NH_{3})_{2}]^{+} as precursors under the same conditions, which therefore exhibit higher photocatalytic activity than spherical nanoparticles [35]. Moreover, the morphologies and structures of the as-prepared Ag_{3}PO_{4} crystals could be further tailored by changing the aging time of the [Ag(NH_{3})_{2}]^{+} complex due to the ammonia volatility. For example, when [Ag(NH_{3})_{2}]^{+} complex solution was aged at room temperature for 1 h, the as-prepared Ag_{3}PO_{4} crystals possess irregular cubic morphology and six rhombic planes. Upon further increasing the aging time up to 2 h, the Ag_{3}PO_{4} crystals transform into irregular structure with concave surfaces. Interestingly, when the aging time has been prolonged to 4 h, the corresponding Ag_{3}PO_{4} products with four symmetrically arrowheaded morphologies have been fabricated (shown in Figure 3), and no cubes have been observed. The variation of morphologies and structures of the as-prepared Ag_{3}PO_{4} crystals leads to the variation of optical properties (Figure 3(d)). Similar morphology variation of Ag_{3}PO_{4} particles prepared by a pyridine-assisted hydrothermal method is found to change regularly from spherical to particles with the corners and edges then to rhombic dodecahedrons with an increase in pyridine concentration [27].

#### 4. Theoretical Study of the Electronic Structure and Photocatalytic Performance

To elucidate its mechanism of the extremely high photooxidative under visible light irradiation of Ag_{3}PO_{4}, theoretical works have been carried out by using first-principle method. Photocatalysis reactions are determined primarily by three processes: (1) the photoexcitation of electron-hole pairs due to light harvesting, (2) the transfer of carriers to the surface, and (3) chemical reactions on the surface. So far, theoretical investigations are mainly focused on the first process, which is relevant to energy band configuration because photoexcited carriers are generated only when the incident photon energy is higher than the bandgap of the photocatalyst. Alignment between the band edges and the redox potentials of the target molecules is also crucial, considering that photoexcited carriers can only be transferred to the adsorbed molecules when there is a sufficiently large negative offset of the conduction band minimum (CBM) and a sufficiently large positive offset of the valence band maximum (VBM) with respect to the redox potentials. Ma et al. investigated the electronic properties and photocatalytic activation of Ag_{3}PO_{4} using first principles density functional theory (DFT) incorporating the local density approximation (LDA) + U formalism [24]. It is found that one PO_{4} tetrahedron and three tetrahedral AgO_{4} are combined with each other through the corner oxygen. The tetrahedral AgO_{4} is heavily distorted to have a dipole moment of 2.2 D (D = debye), which should be closely attributed to a specific nonmetal salt of the oxyacid structure of Ag_{3}PO_{4}. In addition, P ions have a large negative charge which maintains a large dipole in the Ag_{3}PO_{4}, resulting in the distortion of tetrahedral AgO_{4}. As a consequence, a correlation between the photocatalytic activity and the distortion of AgO_{4} tetrahedron is true for a specific phosphate structure. Meanwhile, P possessing a large electron cloud overlapping prefers to attract holes and repel electrons, which helps the e^{-}/h^{+} separation. The calculated results show that Ag_{3}PO_{4} is an indirect band gap semiconductor; the direct band gap is 2.61 eV and the indirect band gap is 2.43 eV having the character of *σ* or *π* bonding states in the VB and the corresponding *σ** or *π** antibonding states in the CB. The effective mass of electrons is far smaller than that of holes, which consequently results in a striking difference of the mobility between photoexcited electrons and holes. This is beneficial for decreasing the recombination of electron-hole pairs in Ag_{3}PO_{4}. In addition, Ag vacancies in Ag_{3}PO_{4} with high concentration have a significant effect on the separation of electron-hole pairs and optical absorbance in the visible-light region. To explore the mechanism of the high performance of Ag_{3}PO_{4}, Umezawa et al. have conducted a comparative study of the electronic structures of Ag_{3}PO_{4}, Ag_{2}O, and AgNbO_{3} by first principles calculations [32]. The CBM consisting of Ag s states in Ag_{3}PO_{4} and Ag d states in Ag_{2}O is the main difference between Ag_{3}PO_{4} and Ag_{2}O, which is due to the rigid PO_{4} tetrahedral unit; partial charge density originating from O sp and P sp derived bonding states is evident in the local density of states (DOS). This increases the ionic character of Ag^{+} and (PO_{4})^{3−}, making the covalent Ag–O bonds weaker. Thus, the hybridization of Ag d and O p states is negligible in Ag_{3}PO_{4}, rendering fully occupied d states at the VBM. On the contrary, covalent Ag–O bonds, that is, antibonding states of Ag d–O p lying at the CBM are formed in Ag_{2}O. In AgNbO_{3}, the majority of the CBM is composed of Nb d states and the nature of the Ag–O bonding does not significantly affect the characteristics of the CBM.

In Figure 4, the band structures of Ag_{3}PO_{4}, Ag_{2}O, and AgNbO_{3} are illustrated, accompanied by the wave function corresponding to the CBM. In Ag_{3}PO_{4}, the wave function at the CBM is dramatically delocalized due to mainly consisting of Ag s states. In contrast, the CBM of Ag_{2}O possesses the character of Ag d–O p antibonding states, which are unfavorable for electron transfer due to their localization. In Ag_{3}PO_{4}, a large amount of hybridization between Ag s states on adjacent atoms leads to a dispersive band structure at the CBM without the “contamination” of d states, resulting in a decreased effective electron mass. In AgNbO_{3}, the CBM mainly composes of and states, causing an anisotropic charge distribution (Figure 4(c)) and allowing electron transfer only along the -direction. This anisotropy can also be found in the band structure, where the dispersion of the CBM is very dispersive along X-S-Y and flat along S-Γ indicating the high dependence of the directions. This is undesirable for photocatalysis process because the limited directionality of the electron transfer leads to higher probability of carrier recombination. The CBM of Ag_{3}PO_{4} has, on the contrary, a very isotropic distribution and is hence favorable for electron transfer (Figure 4(a)). The effective mass of the electron is relatively small in every direction in Ag_{3}PO_{4}, which is also advantageous for electron transfer. Thus, the excellent photocatalytic performance of Ag_{3}PO_{4} is partly due to the highly dispersive band structure at the CBM, which results from Ag s–Ag s hybridization without localized d states.

Using the local density approximation (LDA) and LDA+U approaches, the calculated band gaps of 0.36 and 1.30 eV are far less than the experimental value of 2.45 eV due to the missing discontinuity in the exchange-correlation potential and the self-interaction error within the LDA. To effectively remedy the drawbacks of LDA and understand the photocatalytic mechanism, hybrid density functional theory (DFT) using PBE0 formalism, was used to calculate the band structure, density of state (DOS), and optical properties of Ag_{3}PO_{4} [40]. The hybrid-DFT method gives a direct band gap, eV, and an indirect one, eV, which agrees well with the experimental value (2.45 eV). Compared with the top of valence band (VB), the bottom of conduction band (CB) is well dispersive, which indicates that the photogenerated electrons possess smaller effective mass and, therefore, higher migration ability. The redox ability of Ag_{3}PO_{4} is evaluated by determining the energy positions of valence and conduction bands using Mulliken electronegativity and the band gap value calculated accurately. Figure 5 renders the valence and conduction band edge potentials of Ag_{3}PO_{4}. The VBM potential of Ag_{3}PO_{4} is 2.67 V, more positive than O_{2}/H_{2}O (1.23 V), indicating that Ag_{3}PO_{4} has the ability to oxidize H_{2}O to produce O_{2} or oxidation pollutants. Whereas the CBM potential of Ag_{3}PO_{4} is 0.24 V, which is lesser than H^{+}/H_{2} (0 V) and cannot reduce H^{+} to H_{2} [40]. More recently, Ma et al. investigated the electronic and photocatalytic properties of Ag_{3}P(C = O, S, Se) by the hybrid density functional method. Similar results for Ag_{3}PO_{4} are obtained [41].

#### 5. Visible Light Response Ag_{3}PO_{4} Based Composite Photocatalyst

To harvest photons in visible region, many narrow bandgap metal oxides or chalcogenides have been coupled with TiO_{2} to fabricate visible-light photocatalysts, which exhibit visible-light photocatalytic activity to a certain extent. Such a strategy is also applied to modify Ag_{3}PO_{4} photocatalyst to enhance its photocatalytic activity and/or improve its stability. The previous investigations showed that the photocatalytic activity of Ag_{3}PO_{4} can be enhanced as Ag nanoparticles deposited on Ag_{3}PO_{4} because the Ag_{3}PO_{4} decomposition could capture the photogenerated electrons and thus prevent the recombination of electron-hole pairs within the Ag_{3}PO_{4} samples at the initial stage of photocatalytic reactions. However, the photoactivity decreases with increasing Ag contents due to the formation of Ag layers on the surface of Ag_{3}PO_{4} that shield light absorption, inhibit the transfer of holes from the valance band of Ag_{3}PO_{4} to the interface between photocatalyst, and solution and also hinder the contact of dye molecules with Ag_{3}PO_{4}, and, accordingly, the photocatalytic activity deteriorates gradually [34]. This deterioration of the Ag_{3}PO_{4} photocatalytic activity due to photocorrosion largely limits its practical application as a recyclable highly efficient photocatalyst. It is found that the Ag/Ag_{3}PO_{4} heterocubes synthesized by reacting Ag_{3}PO_{4} cubes with glucose in an aqueous ammonia solution exhibit higher photocatalytic activities than pure Ag_{3}PO_{4} cubes for the organic contaminants degradation under visible-light irradiation [26]. The stability improvement of Ag_{3}PO_{4} by covering Ag^{0} nanoparticles on the surface of Ag_{3}PO_{4} is attributed to the localized surface plasmon resonance (LSPR) effects of silver nanoparticles and a large negative charge of P ions [2, 27], which effectively inhibit the reducibility of Ag^{+} ions in the Ag_{3}PO_{4} lattice. Ag_{3}PO_{4} can also be rejuvenated from weak photocatalytically active Ag as a recyclable highly efficient photocatalyst by oxidizing Ag with H_{2}O_{2} under a P ion atmosphere [29]. However, these strategies are not ideal from the practical application perspective. Thus, the fabrication of Ag_{3}PO_{4} based composite photocatalysts with high photocatalytic activity and excellent stability as well as lower Ag usage for their large scale applications is desirable.

Yao et al. synthesized Ag_{3}PO_{4}/TiO_{2} visible light photocatalyst by depositing of Ag_{3}PO_{4} nanoparticles onto the TiO_{2} (P25) surface photocatalyst [42]. Their results show that the Ag_{3}PO_{4}/TiO_{2} heterostructured photocatalyst shows enhanced activity and is much more stable than unsupported Ag_{3}PO_{4}. The enhanced activity is attributed to the electron-hole effective separation and the larger surface area of the Ag_{3}PO_{4}/TiO_{2} composite, while the enhanced stability is ascribed to the chemical adsorption of Ag^{+} cations in Ag_{3}PO_{4} and O^{−} anions in TiO_{2}. Moreover, the silver weight percentage of the photocatalyst decreases from 77% to 47%, significantly reducing the cost of Ag_{3}PO_{4} based photocatalysts for the Ag_{3}PO_{4}/TiO_{2} composite [42].

The UV photocatalytic activity of Ag_{3}PO_{4}/TiO_{2} composite heterostructures was comparable to that of Ag_{3}PO_{4} nanoparticles surfaces. While the stability and hence reusability of the Ag_{3}PO_{4}/TiO_{2} heterostructure catalysts was substantially enhanced as compared with that of Ag_{3}PO_{4} nanoparticles or TiO_{2} nanobelts alone. These results were attributed to the improved charge separation of the photogenerated electrons and holes under UV light at the Ag_{3}PO_{4}/TiO_{2} interface and/or surfactant-like function of the nanobelts in stabilizing the Ag_{3}PO_{4} nanoparticles. Ag_{3}PO_{4}/TiO_{2} composite heterostructures appear to be more desirable in long-term applications because of their photocatalytic activity as well as the enhanced chemical stability [33].

Considering that the VB level of Ag_{3}PO_{4} is appreciably lower than that of TiO_{2} with +2.7 V (versus NHE) and Ag_{3}PO_{4} can be severed as an appropriate sensitizer for TiO_{2}, Lee et al. fabricated the novel heterojunction structures of Ag_{3}PO_{4}-core/TiO_{2}-shell by covering the Ag_{3}PO_{4} nanoparticles with polycrystalline TiO_{2} by sol-gel method. The prepared Ag_{3}PO_{4}/TiO_{2} composites show notably enhanced photocatalytic activity in decomposing gaseous 2-propanol and evolving CO_{2} compared to bare Ag_{3}PO_{4} and TiO_{2}. It is inferred that the unusually high visible-light photocatalytic activity of Ag_{3}PO_{4}/TiO_{2} composite originates from the unique relative band positions of the two semiconductors [43].

Besides Ag_{3}PO_{4}/TiO_{2} composite heterostructures, AgX/Ag_{3}PO_{4} (X=Cl, Br, I) heterocrystals have also attracted much attention due to the excellent photocatalytic activity. Bi and coworkers [44] have reported that the AgX/Ag_{3}PO_{4} (X=Cl, Br, I) heterocrystals prepared by in situ ionexchange method embodied some advantages compared to the single Ag_{3}PO_{4}, and it is a more promising and fascinating visible-light-driven photocatalyst than pure Ag_{3}PO_{4} [45]. The AgBr/Ag_{3}PO_{4} hybrid synthesized using an in situ anion-exchange method displayed much higher photocatalytic activity than single AgBr or Ag_{3}PO_{4}, as well as high stability under visible light irradiation. The high stability was attributed to the formed Ag@AgBr/Ag_{3}PO_{4}@Ag plasmonic system, which effectively retains its activity due to the efficient transfer of photoinduced electrons [45].

#### 6. Conclusion and Perspectives

In this paper, we have summarized the survey of efforts on Ag_{3}PO_{4} photocatalysts. As a quintessence, for example, Ag_{3}PO_{4} photocatalysts have excellent photocatalytic activity and yield a high quantum yield of nearly 90% under visible light ( nm) found for the evolution of O_{2} in water photolysis [23]. All of the developments show that Ag_{3}PO_{4} and/or its heterogeneous composites have the potential as excellent visible-light-active candidates with high photocatalytic activity. However, to comply with the challenging requirements of economically viable industrial production, many issues are still yet to be addressed, including long-term stability of Ag_{3}PO_{4} in photocatalytic processes. New methods for fabrication Ag_{3}PO_{4} with exposed high-energy facets and novel heterogeneous Ag_{3}PO_{4} cocatalysts are highly desirable. To date, there have been relatively few quantitative studies in the charge carrier dynamics in Ag_{3}PO_{4} and/or its cocatalysts systems, how these dynamics are related to material design, and how they impact the photocatalytic processes. In heterogeneous systems, a particular challenge is that electron-hole recombination is a bimolecular process, which its dynamics often depend nonlinearly on the charge carrier density and so cannot be described using a single time constant. Therefore, obtaining a substantial breakthrough in efficiency requires an exact understanding of the surface/interface processes at the atomic scale. A true picture of photocatalyst surfaces in action, including such recombination dynamics, needs to be studied by in situ observations using transient optical spectroscopy techniques. A further challenge is translating laboratory-scale academic research into scalable, manufacturable technologies to meet the demands of the efficient utilization of solar energy in the areas of renewable energy and environmental purification.

#### Acknowledgments

This work is supported by the Hunan Provincial Natural Science Foundation of China (Grant no. 12JJ3009), the Science and Technology Plan Projects of Hunan Province (2012ZK3021).

#### References

- L. W. Zhang, Y. Man, and Y. F. Zhu, “Effects of Mo replacement on the structure and visible-light-induced photocatalytic performances of Bi
_{2}WO_{6}photocatalyst,”*ACS Catalysis*, vol. 1, no. 8, pp. 841–848, 2011. View at Publisher · View at Google Scholar · View at Scopus - Y. P. Liu, L. Fang, H. D. Lu, L. J. Liu, H. Wang, and C. Z. Hu, “Highly efficient and stable Ag/Ag
_{3}PO_{4}plasmonic photocatalyst in visible light,”*Catalysis Communications*, vol. 17, pp. 200–204, 2012. View at Publisher · View at Google Scholar - R. Asahi, T. Morikawa, T. Ohwaki, et al., “Photocatalysts sensitive to visible light,”
*Science*, vol. 295, no. 5555, pp. 626–627, 2002. View at Publisher · View at Google Scholar · View at Scopus - G. S. Wu, J. L. Wen, S. Nigro, and A. C. Chen, “One-step synthesis of N-and F-codoped mesoporous TiO
_{2}photocatalysts with high visible light activity,”*Nanotechnology*, vol. 21, no. 8, Article ID 085701, 2010. View at Publisher · View at Google Scholar · View at Scopus - Y. Tian, G. F. Huang, L. J. Tang, M. G. Xia, W. Q. Huang, and Z. L. Ma, “Size-controllable synthesis and enhanced photocatalytic activity of porous ZnS nanospheres,”
*Materials Letters*, vol. 83, pp. 104–107, 2012. View at Publisher · View at Google Scholar - Y. Chen, G. F. Huang, W. Q. Huang, B. S. Zou, and A. L. Pan, “Enhanced visible-light photoactivity of La-doped ZnS thin films,”
*Applied Physics A*, vol. 108, no. 4, pp. 895–900, 2012. View at Publisher · View at Google Scholar - V. Etacheri, M. K. Seery, S. J. Hinder, and S. C. Pillai, “Highly visible light active TiO
_{2-x}N_{x}heterojunction photocatalysts,”*Chemistry of Materials*, vol. 22, no. 13, pp. 3843–3853, 2010. View at Publisher · View at Google Scholar · View at Scopus - L. Feng, K. F. He, and W. P. Chen, “Study on stability of AgI/TiO
_{2}visible light photocatalysts in solutions of various pH values,”*New Materials, Applications and Processes*, vol. 399-401, pp. 1272–1275, 2012. View at Google Scholar - J. J. Yuan, H. D. Li, S. Y. Gao, Y. H. Lin, and H. Y. Li, “A facile route to n-type TiO
_{2}-nanotube/p-type boron-doped-diamond heterojunction for highly efficient photocatalysts,”*Chemical Communications*, vol. 46, no. 18, pp. 3119–3121, 2010. View at Publisher · View at Google Scholar · View at Scopus - J. Q. Li, D. F. Wang, Z. Y. Guo, and Z. F. Zhu, “Preparation, characterization and visible-light-driven photocatalytic activity of Fe-incorporated TiO
_{2}microspheres photocatalysts,”*Applied Surface Science*, vol. 263, pp. 382–388, 2012. View at Publisher · View at Google Scholar - Y. Komai, K. Okitsu, R. Nishimura et al., “Visible light response of nitrogen and sulfur co-doped TiO
_{2}photocatalysts fabricated by anodic oxidation,”*Catalysis Today*, vol. 164, no. 1, pp. 399–403, 2011. View at Publisher · View at Google Scholar · View at Scopus - X. M. Fang, Z. G. Zhang, and Q. L. Chen, “Nitrogen doped TiO
_{2}photocatalysts with visible-light activity,”*Progress in Chemistry*, vol. 19, no. 9, pp. 1282–1290, 2007. View at Google Scholar · View at Scopus - Y. Hu, D. Z. Li, Y. Zheng et al., “BiVO
_{4}/TiO_{2}nanocrystalline heterostructure: a wide spectrum responsive photocatalyst towards the highly efficient decomposition of gaseous benzene,”*Applied Catalysis B*, vol. 104, no. 1-2, pp. 30–36, 2011. View at Publisher · View at Google Scholar · View at Scopus - Y. J. Chen, Y. Q. Zhang, C. Liu, A. M. Lu, and W. H. Zhang, “Photodegradation of malachite green by nanostructured Bi
_{2}WO_{6}visible light-induced photocatalyst,”*International Journal of Photoenergy*, vol. 2012, Article ID 510158, 6 pages, 2012. View at Publisher · View at Google Scholar - J. W. Tang, Z. G. Zou, and J. H. Ye, “Efficient photocatalytic decomposition of organic contaminants over CaBi
_{2}O_{4}under visible-light irradiation,”*Angewandte Chemie*, vol. 43, no. 34, pp. 4463–4466, 2004. View at Publisher · View at Google Scholar · View at Scopus - H. G. Kim, P. H. Borse, J. S. Jang, E. D. Jeong, and J. S. Lee, “Enhanced photochemical properties of electron rich W-doped PbBi
_{2}Nb_{2}O_{9}layered perovskite material under visible-light irradiation,”*Materials Letters*, vol. 62, no. 8-9, pp. 1427–1430, 2008. View at Publisher · View at Google Scholar · View at Scopus - T. P. Cao, Y. J. Li, C. H. Wang et al., “Bi
_{4}Ti_{3}O_{12}nanosheets/TiO_{2}submicron fibers heterostructures: in situ fabrication and high visible light photocatalytic activity,”*Journal of Materials Chemistry*, vol. 21, no. 19, pp. 6922–6927, 2011. View at Publisher · View at Google Scholar · View at Scopus - D. L. Chen, S. H. Yoo, Q. S. Huang, G. Ali, and S. O. Cho, “Sonochemical synthesis of Ag/AgCl nanocubes and their efficient visible-light-driven photocatalytic performance,”
*Chemistry A*, vol. 18, no. 17, pp. 5192–5200, 2012. View at Publisher · View at Google Scholar - M. Kitano, M. Matsuoka, M. Ueshima, and M. Anpo, “Recent developments in titanium oxide-based photocatalysts,”
*Applied Catalysis A*, vol. 325, no. 1, pp. 1–14, 2007. View at Publisher · View at Google Scholar · View at Scopus - L. Xu, C. Li, W. Shi, J. Guan, and Z. Sun, “Visible light-response NaTa
_{1-x}Cu_{x}O_{3}photocatalysts for hydrogen production from methanol aqueous solution,”*Journal of Molecular Catalysis A*, vol. 360, pp. 42–47, 2012. View at Publisher · View at Google Scholar - R. Niishiro, H. Kato, and A. Kudo, “Nickel and either tantalum or niobium-codoped TiO
_{2}and SrTiO_{3}photocatalysts with visible-light response for H_{2}or O_{2}evolution from aqueous solutions,”*Physical Chemistry Chemical Physics*, vol. 7, no. 10, pp. 2241–2245, 2005. View at Publisher · View at Google Scholar · View at Scopus - W. Xiong, Q. D. Zhao, X. Y. Li, and D. K. Zhang, “One-step synthesis of flower-like Ag/AgCl/BiOCl composite with enhanced visible-light photocatalytic activity,”
*Catalysis Communications*, vol. 16, no. 1, pp. 229–233, 2011. View at Publisher · View at Google Scholar - Z. G. Yi, J. H. Ye, N. Kikugawa et al., “An orthophosphate semiconductor with photooxidation properties under visible-light irradiation,”
*Nature Materials*, vol. 9, no. 7, pp. 559–564, 2010. View at Publisher · View at Google Scholar · View at Scopus - X. G. Ma, B. Lu, D. Li, R. Shi, C. S. Pan, and Y. F. Zhu, “Origin of photocatalytic activation of silver orthophosphate from first-principles,”
*Journal of Physical Chemistry C*, vol. 115, no. 11, pp. 4680–4687, 2011. View at Publisher · View at Google Scholar · View at Scopus - H. N. Ng, C. Calvo, and R. Faggiani, “A new investigation of the structure of silver orthophosphate,”
*Acta Crystallographica B*, vol. 34, no. 3, pp. 898–899, 1978. View at Publisher · View at Google Scholar - Y. P. Bi, H. Y. Hu, S. X. Ouyang, Z. B. Jiao, G. X. Lu, and J. H. Ye, “Selective growth of metallic Ag nanocrystals on Ag
_{3}PO_{4}submicro-cubes for photocatalytic applications,”*Chemistry A*, vol. 18, no. 45, pp. 14272–14275, 2012. View at Publisher · View at Google Scholar - Y. P. Liu, L. Fang, H. D. Lu, Y. W. Li, C. Z. Hu, and H. G. Yu, “One-pot pyridine-assisted synthesis of visible-light-driven photocatalyst Ag/Ag
_{3}PO_{4},”*Applied Catalysis B*, vol. 115-116, pp. 245–252, 2012. View at Publisher · View at Google Scholar - G. P. Li and L. Q. Mao, “Magnetically separable Fe
_{3}O_{4}-Ag_{3}PO_{4}sub-micrometre composite: facile synthesis, high visible light-driven photocatalytic efficiency, and good recyclability,”*RSC Advances*, vol. 2, no. 12, pp. 5108–5111, 2012. View at Publisher · View at Google Scholar - H. Wang, Y. S. Bai, J. T. Yang, X. F. Lang, J. H. Li, and L. Guo, “A facile way to rejuvenate Ag
_{3}PO_{4}as a recyclable highly efficient photocatalyst,”*Chemistry A*, vol. 18, no. 18, pp. 5524–5529, 2012. View at Publisher · View at Google Scholar - Y. Bi, S. Ouyang, N. Umezawa, J. Cao, and J. Ye, “Facet effect of single-crystalline Ag
_{3}PO_{4}sub-microcrystals on photocatalytic properties,”*Journal of the American Chemical Society*, vol. 133, no. 17, pp. 6490–6492, 2011. View at Publisher · View at Google Scholar · View at Scopus - H. C. Zhang, H. Huang, H. Ming et al., “Carbon quantum dots/Ag
_{3}PO_{4}complex photocatalysts with enhanced photocatalytic activity and stability under visible light,”*Journal of Materials Chemistry*, vol. 22, no. 21, pp. 10501–10506, 2012. View at Publisher · View at Google Scholar - N. Umezawa, O. Y. Shuxin, and J. H. Ye, “Theoretical study of high photocatalytic performance of Ag
_{3}PO_{4},”*Physical Review B*, vol. 83, no. 3, Article ID 035202, 2011. View at Publisher · View at Google Scholar · View at Scopus - R. Y. Liu, P. G. Hu, and S. W. Chen, “Photocatalytic activity of Ag
_{3}PO_{4}nanoparticle/TiO_{2}nanobelt heterostructures,”*Applied Surface Science*, vol. 258, no. 24, pp. 9805–9809, 2012. View at Publisher · View at Google Scholar - W. G. Wang, B. Cheng, J. G. Yu, G. Liu, and W. H. Fan, “Visible-light photocatalytic activity and deactivation mechanism of Ag
_{3}PO_{4}spherical particles,”*Chemistry*, vol. 7, no. 8, pp. 1902–1908, 2012. View at Publisher · View at Google Scholar - Y. P. Bi, H. Y. Hu, S. X. Ouyang, G. X. Lu, J. Y. Cao, and J. H. Ye, “Photocatalytic and photoelectric properties of cubic Ag
_{3}PO_{4}sub-microcrystals with sharp corners and edges,”*Chemical Communications*, vol. 48, no. 31, pp. 3748–3750, 2012. View at Publisher · View at Google Scholar - M. Ge, N. Zhu, Y. P. Zhao, J. Li, and L. Liu, “Sunlight-assisted degradation of dye pollutants in Ag
_{3}PO_{4}suspension,”*Industrial & Engineering Chemistry Research*, vol. 51, no. 14, pp. 5167–5173, 2012. View at Publisher · View at Google Scholar - Z. B. Jiao, Y. Zhang, H. C. Yu, G. X. Lu, J. H. Ye, and Y. P. Bi, “Concave trisoctahedral Ag
_{3}PO_{4}microcrystals with high-index facets and enhanced photocatalytic properties,”*Chemical Communications*, vol. 49, no. 6, pp. 636–638, 2013. View at Publisher · View at Google Scholar - J. Wang, F. Teng, M. D. Chen, J. J. Xu, Y. Q. Song, and X. L. Zhou, “Facile synthesis of novel Ag
_{3}PO_{4}tetrapods and the {110} facets-dominated photocatalytic activity,”*Crystengcomm*, vol. 15, no. 1, pp. 39–42, 2013. View at Publisher · View at Google Scholar - C. T. Dinh, T. D. Nguyen, F. Kleitz, and T. O. Do, “Large-scale synthesis of uniform silver orthophosphate colloidal nanocrystals exhibiting high visible light photocatalytic activity,”
*Chemical Communications*, vol. 47, no. 27, pp. 7797–7799, 2011. View at Publisher · View at Google Scholar · View at Scopus - J. J. Liu, X. L. Fu, S. F. Chen, and Y. F. Zhu, “Electronic structure and optical properties of Ag
_{3}PO_{4}photocatalyst calculated by hybrid density functional method,”*Applied Physics Letters*, vol. 99, Article ID 191903, 3 pages, 2011. View at Publisher · View at Google Scholar - Z. J. Ma, Z. G. Yi, J. Sun, and K. C. Wu, “Electronic and photocatalytic properties of Ag
_{3}PC_{4}VI (C = O, S, Se): a systemic hybrid DFT study,”*The Journal of Physical Chemistry C*, vol. 116, no. 47, pp. 25074–25080, 2012. View at Publisher · View at Google Scholar - W. F. Yao, B. Zhang, C. P. Huang, C. Ma, X. L. Song, and Q. J. Xu, “Synthesis and characterization of high efficiency and stable Ag
_{3}PO_{4}/TiO_{2}visible light photocatalyst for the degradation of methylene blue and rhodamine B solutions,”*Journal of Materials Chemistry*, vol. 22, no. 9, pp. 4050–4055, 2012. View at Publisher · View at Google Scholar - S. B. Rawal, S. D. Sung, and W. I. Lee, “Novel Ag
_{3}PO_{4}/TiO_{2}composites for efficient decomposition of gaseous 2-propanol under visible-light irradiation,”*Catalysis Communications*, vol. 17, pp. 131–135, 2012. View at Publisher · View at Google Scholar - Y. P. Bi, S. X. Ouyang, J. Y. Cao, and J. H. Ye, “Facile synthesis of rhombic dodecahedral AgX/Ag
_{3}PO_{4}(X = Cl, Br, I) heterocrystals with enhanced photocatalytic properties and stabilities,”*Physical Chemistry Chemical Physics*, vol. 13, no. 21, pp. 10071–10075, 2011. View at Publisher · View at Google Scholar · View at Scopus - J. Cao, B. D. Luo, H. L. Lin, B. Y. Xu, and S. F. Chen, “Visible light photocatalytic activity enhancement and mechanism of AgBr/Ag
_{3}PO_{4}hybrids for degradation of methyl orange,”*Journal of Hazardous Materials*, vol. 217, pp. 107–115, 2012. View at Publisher · View at Google Scholar